Published on Web 06/18/2008
Amphiphilic Molecular Design as a Rational Strategy for Tailoring Bicontinuous Electron Donor and Acceptor Arrays: Photoconductive Liquid Crystalline Oligothiophene-C60 Dyads Wei-Shi Li,*,† Yohei Yamamoto,† Takanori Fukushima,*,†,‡ Akinori Saeki,§ Shu Seki,§ Seiichi Tagawa,§ Hiroyasu Masunaga,# Sono Sasaki,# Masaki Takata,#,| and Takuzo Aida*,†,‡ ERATO-SORST Nanospace Project, Japan Science and Technology Agency (JST), National Museum of Emerging Science and InnoVation, 2-41 Aomi, Koto-ku, Tokyo 135-0064, Japan, Department of Chemistry and Biotechnology, School of Engineering and Center for NanoBio Integration, The UniVersity of Tokyo, 7-3-1 Hongo, Bunkyo-ku, Tokyo 113-8656, Japan, Institute of Scientific and Industrial Research (ISIR), Osaka UniVersity, 8-1, Mihogaoka, Ibaraki, Osaka 567-0047, Japan, Japan Synchrotron Radiation Research Institute (JASRI), 1-1-1 Kouto, Sayo-cho, Sayo-gun, Hyogo 679-5198, Japan, and RIKEN SPring-8 Center, 1-1-1 Kouto, Sayo-cho, Sayo-gun, Hyogo 679-5148, Japan Received April 15, 2008; E-mail: [email protected]
; [email protected]
; [email protected]
Tailoring bicontinuous electron donor (D) and acceptor (A) arrays in solution-processable materials is an essential step for the realization of thin-film organic optoelectronics.1 Casting of a D/A mixture may give rise to photoconductive bulk materials.2 However, without proper choice of the components, many defects are usually formed, leading to trapping and rapid annihilation of charge carriers. In view of photovoltaics, the presence of bicontinuous D and A arrays is essential, but cast films from D/A mixtures likely contain their charge-transfer complexes. So far, nanofibers and tubes with bicontinuous D and A arrays have been obtained by self-assembly of covalently linked D-A dyads.3,4 Nevertheless, solution-processable bulk materials with a D/A heterojunction5 might be more realistic for device applications. Here we report a photoconductive liquid crystal (LC) with bicontinuous arrays of densely packed D and A components, tailored from amphiphilic oligothiophene-C60 dyad 1Amphi (Chart 1).6 Together with contrasting results for a nonamphiphilic reference (1Lipo), we highlight a crucial role of the amphiphilic design both in structuring and in photoconductivity. The molecular structures of 1Amphi and 1Lipo are identical to each other except for the terminal wedges. 1Amphi bears a hydrophilic wedge with triethylene glycol chains and, on the other side, a hydrophobic wedge with paraffinic chains. In contrast, 1Lipo possesses only the paraffinic wedges. We also prepared compounds 2 and 3, which are equivalent to the donor and acceptor components of 1Amphi, respectively. They are all soluble in CH2Cl2, where the absorption spectral profiles (Figure S3) and redox properties (Figure S4) of 1Amphi and 1Lipo were essentially identical to one another.6 Dyad 1Amphi formed a LC smectic A mesophase over a wide temperature range from 136.1 to 18.3 °C (Figure S5).6 Polarized optical microscopy (POM) of LC-1Amphi displayed a typical focalconic texture (Figure 1a). Synchrotron radiation small-angle X-ray scattering (SAXS) analysis showed sharp peaks with d spacings of 10.6, 5.3, 3.5, and 2.6 nm (Figure 1c), which can be indexed as (100), (200), (300), and (400) reflections of a lamellar structure with a layer width of 10.6 nm. On the basis of a CPK model of 1Amphi, the observed layer width is almost twice as large as the distance from the paraffinic end to the fullerene unit (∼5.5 nm;
Chart 1. Structures of 1Amphi, 1Lipo, and References 2 and 3
Figure 2, I). Thus, each repeating layer consists of laterally coupled tail-to-tail pairs of 1Amphi, and such layers are connected at the fullerene-appended hydrophilic head part of 1Amphi to form a 2D lamellar structure. In this configuration, the hydrophilic and paraffinic wedges are separated by 5.3 nm. Similar to 1Amphi, nonamphiphilic 1Lipo formed a smectic A LC mesophase in a temperature range from 111.4 to 12.5 °C, as
ERATO-SORST Nanospace Project, JST. The University of Tokyo. Osaka University. # JASRI. | RIKEN. ‡ §
J. AM. CHEM. SOC. 2008, 130, 8886–8887
Figure 1. POMs at 33 °C and SAXS patterns at 30 °C (inset: magnified at q ) 1.5-2.5 nm-1) of (a,c) LC-1Amphi and (b,d) LC-1Lipo. 10.1021/ja802757w CCC: $40.75 2008 American Chemical Society
Figure 2. Schematic representations of molecular orientations in LC-1Amphi
(I) and LC-1Lipo (II) with a smectic A mesophase.
mixture of 2 and 3 formed neither regular structures nor photoconductivity (black). Noteworthy, LC-1Lipo (red) was much less conductive than LC-1Amphi, where the photocurrent was only 1/10 that of 1Amphi observed under identical conditions. This result is interesting since the electron transfer efficiencies in LC-1Amphi and LC-1Lipo, judging from their fluorescence quenching profiles (Figure S6),6 are considered equally high. Having these features in mind, we conducted flash photolysis time-resolved microwave conductivity (FR-TRMC) measurements, which are informative of the behaviors of mobile charge carriers in a short distance (∼10 nm). With a 355 nm laser pulse at 25 °C (Figure 3d), the maximum conductivity (φΣµmax in cm2/V · s) of LC-1Amphi (4.1 × 10-4) was markedly greater than that of the 2/3 mixture (1.2 × 10-4) but almost comparable to that of LC-1Lipo (3.7 × 10-4). However, the charge carrier, generated in LC-1Lipo, was shorter-lived than that in LC-1Amphi, suggesting the presence of a larger number of trapping sites in LC-1Lipo. This is in accord with the aforementioned low structural integrity of LC-1Lipo (Figure 2, II) and its poor photoconducting nature in a macroscopic scale (Figure 3b). In summary, we have demonstrated that amphiphilic molecular design7 can be a rational strategy for the spontaneous formation of bicontinuous donor and acceptor arrays in liquid crystalline materials. Site-specific modification of donor-acceptor dyads with hydrophilic and paraffinic wedges not only prohibits donor-acceptor interactions leading to the trapping of charge carriers but also ensures a long-range conducting pathway in the materials. As liquid crystals are solution-processable and self-healable, our design strategy may contribute to the development of high-performance organic optoelectronics. Acknowledgment. The synchrotron radiation experiments were carried out on the BL40B2 of SPring-8 under the Priority Nanotechnology Support Program administrated by JASRI (Proposal No. 2008A1650).
Figure 3. (a) Absorption spectra at 25 °C of 1Amphi (blue) and 1Lipo (red)
in the LC state (solid curves) and in CH2Cl2 (broken curves), normalized at 450 nm. Photoconducting properties at 25 °C of LC-1Amphi (blue), LC1Lipo (red), and a 1:1 mixture of 2 and 3 (black); (b) I-V profiles without (broken curves) and with photoirradiation (solid curves) and (c) changes in photogenerated electric current under an applied voltage of +1 V. (d) FPTRMC profiles (λex ) 355 nm) of LC-1Amphi (blue) and LC-1Lipo (red).
observed by DSC and POM profiles (Figures 1b and S5).6 SAXS pattern (Figure 1d) displayed intense and weak diffractions with d spacings of 5.7 and 2.9 nm, respectively, which were indexed as (100) and (200) reflections of a lamellar structure with a layer width of 5.7 nm (Figure 2, II). The observed width is close to the molecular length of 1Lipo. Considering that both ends of 1Lipo are paraffinic, the head/tail orientation of 1Lipo in the lamellar structure is most likely nonuniform (Figure 2, II). In relation to these structural aspects, the absorption spectrum of LC-1Lipo was different from that of LC-1Amphi, while both were obviously broader than those in CH2Cl2 (Figure 3a). In particular, a broad band observed for LC-1Lipo at 600-800 nm suggests a charge-transfer interaction between the oligothiophene and fullerene units, which can occur unless 1Lipo adopts a uniform head/tail orientation. As shown in Figure 3b,c, LC-1Amphi (blue) exhibited a distinct photoconductive character. At an applied voltage of, for example, +2 V, the current at 25 °C increased abruptly from 0.09 to 26 pA (on/off ratio ) 290) upon irradiation and quickly retrieved the original value when the light was turned off. In contrast, a 1:1
Supporting Information Available: Details of synthesis and characterization of 1Amphi, 1Lipo, 2, and 3, and supporting Figures S1-S6. This material is available free of charge via the Internet at http:// pubs.acs.org. References (1) (a) Segura, J. L.; Martı´n, N.; Guldi, D. M. Chem. Soc. ReV. 2005, 34, 31– 47. (b) Gu¨nes, S.; Neugebauer, H.; Sariciftci, N. S. Chem. ReV. 2007, 107, 1324–1338. (c) Thompson, B. C.; Fre´chet, J. M. J. Angew. Chem., Int. Ed. 2008, 47, 58–77. (2) (a) Percec, V.; Glodde, M.; Bera, T. K.; Miura, Y.; Shiyanovskaya, I.; Singer, K. D.; Balagurusamy, V. S. K.; Heiney, P. A.; Schnell, I.; Rapp, A.; Spiess, H.-W.; Hudsonk, S. D.; Duank, H. Nature 2002, 419, 384–387. (b) SchmidtMende, L.; Fechtenko¨tter, A.; Mu¨llen, K.; Moons, E.; Friend, R. H.; MacKenzie, J. D. Science 2006, 293, 1119–1122. (c) Liscio, A.; De Luca, G.; Nolde, F.; Palermo, V.; Mu¨llen, K.; Samorı`, P. J. Am. Chem. Soc. 2008, 130, 780–781. (3) (a) Yamamoto, Y.; Fukushima, T.; Suna, Y.; Ishii, N.; Saeki, A.; Seki, S.; Tagawa, S.; Taniguchi, M.; Kawai, T.; Aida, T. Science 2006, 314, 1761– 1764. (b) Yamamoto, Y.; Fukushima, T.; Saeki, A.; Seki, S.; Tagawa, S.; Ishii, N.; Aida, T. J. Am. Chem. Soc. 2007, 129, 9276–9277. (4) (a) Wu¨rthner, F.; Chen, Z.; Hoeben, F; J, M.; Osswald, P.; You, C.-C.; Jonkheijm, P.; Herrikhuyzen, J. v.; Schenning, A. P. H. J.; van der Schoot, P. P. A. M.; Meijer, E. W.; Beckers, E. H. A.; Meskers, S. C. J.; Janssen, R. A. J. J. Am. Chem. Soc. 2004, 126, 10611–10618. (b) Ro¨ger, C.; Mu¨ller, M. G.; Lysetska, M.; Miloslavina, Y.; Holzwarth, A. R.; Wu¨rthner, F. J. Am. Chem. Soc. 2006, 128, 6542–6543. (5) (a) Samorı`, P.; Yin, X.; Tchebotareva, N.; Wang, Z.; Pakula, T.; Jackel, F.; Watson, M. D.; Venturini, A.; Mu¨llen, K.; Rabe, J. P. J. Am. Chem. Soc. 2004, 126, 3567–3575. (b) Peeters, E.; van Hal, P. A.; Meskers, S. C. J.; Janssen, R. A. J.; Meijer, E. W. Chem.—Eur. J. 2002, 8, 4470–4474. (6) See Supporting Information. (7) For review, see: Tschierske, C. J. Mater. Chem. 2001, 11, 2647–2671.
J. AM. CHEM. SOC.
VOL. 130, NO. 28, 2008